Phase transformations in cast duplex stainless steels 2004
Phase transformations in cast duplex stainless steels Yoon-Jun Kim Iowa State University
Follow this and additional works at: https://lib.dr.iastate.edu/rtd
Part of the Materials Science and Engineering Commons
This Dissertation is brought to you for free and open access by the Iowa State University Capstones, Theses and Dissertations at Iowa State University Digital Repository. It has been accepted for inclusion in Retrospective Theses and Dissertations by an authorized administrator of Iowa State University Digital Repository. For more information, please contact [email protected]
Recommended Citation Kim, Yoon-Jun, "Phase transformations in cast duplex stainless steels " (2004). Retrospective Theses and Dissertations. 1175. https://lib.dr.iastate.edu/rtd/1175
in partial fulfillment of the requirements for the degree of
DOCTOR OF PHILOSOPHY
Program of Study Committee: L. Scott Chumbley, Co-major Professor
Brian Gleeson, Co-major Professor Alan M. Russell
Matthew J. Kramer Frank E. Peters
Iowa State University
UMI Number: 3158349
INFORMATION TO USERS
The quality of this reproduction is dependent upon the quality of the copy
submitted. Broken or indistinct print, colored or poor quality illustrations and
photographs, print bleed-through, substandard margins, and improper
alignment can adversely affect reproduction.
In the unlikely event that the author did not send a complete manuscript
and there are missing pages, these will be noted. Also, if unauthorized
copyright material had to be removed, a note will indicate the deletion.
UMI UMI Microform 3158349
All rights reserved. This microform edition is protected against
unauthorized copying under Title 17, United States Code.
ProQuest Information and Learning Company 300 North Zeeb Road
P.O. Box 1346 Ann Arbor, Ml 48106-1346
This is to certify that the doctoral dissertation of
2.1. Phase Equilibria and Properties of Iron-based Alloys 4
2.1.1. Iron-Carbon Alloys (Fe-FegC Metastable System) 4
2.1.2. Effects of Alloying Additions on Iron-Carbon Alloys 6
2.1.3. Stainless Steels 9
2.2. Basics of Solid State Phase Transformations 14
2.2.1. Factors Affecting Phase Transformations 14
126.96.36.199. Diffusion 14
2.3. Metallurgy and Properties of Cast Duplex Stainless Steels 29
2.3.1. Designations of Cast Stainless Steels 29
2.3.2. Microstructure 30
2.3.3. TTT and CCT Diagrams of Duplex Stainless Steels 33
CHAPTER 3. PROJECT AIMS 37
CHAPTER 4. EXPERIMENTAL PROCEDURES 38
4.1. Sample Preparation 38
4.1.1. TTT Samples 38
4.1.2. CCT Samples 41
4.2. Sample Characterization 44
CHAPTER 5. CHARACTERIZATIONS 48
6.1. Introduction 79
7.1. Modified JMA Anlaysis for CCT Prediction 90
7.2. Microstructures of CD3MN and CD3MWCuN After Cooling 94
7.3. Hardness Testing
CHAPTER 9. GENERAL CONCLUSIONS
Duplex stainless steels (DSS) constitute both ferrite and austenite as a matrix. Such a
microstructure confers a high corrosion resistance with favorable mechanical properties.
However, intermetallic phases such as sigma (a) and chi (%) can also form during casting or
high-temperature processing and can degrade the properties of the DSS. This research was
initiated to develop time-temperature-transformation (TTT) and continuous-cooling-
transformation (CCT) diagrams of two types of cast duplex stainless steels, CD3MN (Fe-
22Cr-5Ni-Mo-N) and CD3MWCuN (Fe-25Cr-7Ni-Mo-W-Cu-N), in order to understand the
time and temperature ranges for intermetallic phase formation. The alloys were heat treated
isothermally or under controlled cooling conditions and then characterized using
conventional metallographic methods that included tint etching, and also using electron
microscopy (SEM, TEM) and wavelength dispersive spectroscopy (WDS). The kinetics of
intermetallic-phase (a + %) formation were analyzed using the Johnson-Mehl-Avrami (JMA)
equation in the case of isothermal transformations and a modified form of this equation in the
case of continuous cooling transformations. The rate of intermetallic-phase formation was
found to be much faster in CD3MWCuN than CD3MN due mainly to differences in the
major alloying contents such as Cr, Ni and Mo. To examine in more detail the effects of
these elements of the phase stabilities, a series of eight steel castings was designed with the
Cr, Ni and Mo contents systematically varied with respect to the nominal composition of
CD3MN. The effects of varying the contents of alloying additions on the formation of
intermetallic phases were also studied computationally using the commercial thermodynamic
software package, Thermo-Calc. In general, a was stabilized with increasing Cr addition and
1 by increasing Mo addition. However, a delicate balance among Ni and other minor
elements such as N and Si also exists. Phase equilibria in DSS can be affected by local
composition fluctuations in the cast alloy. This may cause discrepancy between
thermodynamic prediction and experimental observation.
CHAPTER 1: GENERAL INTRODUCTION
Duplex stainless steels (DSS) constitute a set of steels possessing a nearly equal
amount of the ferrite (S-Fe) and austenite (y-Fe) phases as a matrix. Commercial duplex
stainless steels originated in 1933 when the J. Holtzer Company, a French firm, mistakenly
made an alloy containing 20%Cr-8%Ni-2.5%Mo rather than the target alloy of 18%Cr-
9%Ni-2.5%Mo. Upon investigation of the new alloy, which consisted of a high volume
fraction of ferrite in an austenite matrix, it was found that it possessed high intergranular
corrosion resistance under various environments. Firms in other countries, such as Sweden
and the United States, started to research and produce DSS beginning from the 1940's.
The austenite+ferrite matrix is attainable by combining various phase stabilizing
elements. Cr and Mo are effective ferrite stabilizers, producing a wide ferrite field in phase
diagrams. In general, stainless steels having ferrite as the predominant phase have excellent
corrosion resistance due to the high solubility of Cr in ferrite. On the other hand, Ni and N,
which are effective austenite stabilizers, increase the austenite region in Fe-based systems
and are known to improve mechanical properties. Thus, a structure including high Cr, Mo,
Ni and N will produce a favorable combination of mechanical properties and high corrosion
resistance. The effect produced by these alloying elements on corrosion resistance is
indicated by the pitting resistance equivalent number (PREN) as shown in Eq. 1. The higher
the PREN the better the predicted corrosion properties of a DSS. Alloys having a PREN
greater than 40 are categorized as superduplex grade DSS (Fig. 1).
PREN = %Cr + 3.3 x %Mo +17 x %N Eq. 1
• SAP 2507 • ZERON 100
! UNS 32304
Fig. 1. Nominal PREN values for different stainless steels.[l'
DSS alloys are widely used for their high corrosion resistance in severe corrosive
aqueous environments at service temperatures up to about 800°C. Both wrought and cast
DSS alloys are available depending on the application. A tremendous amount of literature
has been published regarding the phase transformation behavior, alloying element effects,
corrosion resistance and mechanical properties of wrought DSS. However, even though cast
DSS are used in many applications, they have been the subject of little research. It should be
expected that the phase equilibria are different in the cast and wrought alloys due to
differences in their nominal compositions.
The research undertaken in this study was to develop time-temperature-
transformation (TTT, also known as isothermal transformation or IT) diagrams and
continuous-cooling-transformation (CCT) diagrams for two types of cast DSS alloys,
designated CD3MN and CD3MWCuN by the Alloy Casting Institute (ACI). Phase
transformations in these alloys follow a nucleation and growth mechanism that is diffusion
controlled. The transformation kinetics and phase constituents that occur as a result of
quenching followed by isothermal holds were examined and directly measured by optical
analysis using standard metallographic techniques. The phase transformation kinetics for
both isothermal hold and continuous cooled alloys were analyzed from the experimental data
using Johnaon-Mehl-Avrami (JMA) analysis.
The effects of alloying elements on the phase transformations during heat treatment
were interpreted with the aid of the commercial thermodynamic package, Thermo-Calc.
Thermo-Calc enables one to determine phase equilibria of metallic systems by using the
appropriate thermodynamic databases included in the package.
2.1.1. Iron-Carbon Alloys (Fe-FesC Metastable System)
The iron-carbon alloy system represents the basis of steels. The reasons for the
importance of carbon steels are that they are easily and inexpensively produced and possess a
favorable mixture of mechanical properties such as strength, toughness, and ductility by
means of casting, machining and heat treating. Such a combination of properties and
inexpensive price makes carbon steels attractive in industries and markets. However, the
crucial disadvantage of plain-carbon steels is their poor corrosion resistance. Corrosion can
be slowed by painting, enameling, or by appropriate alloying additions, such as Cr. When
added to a level greater than about 10.5 wt.%, Cr protects steels from oxidation ("rust") by
forming a continuous, Cr-rich passive layer on the metal surface.
The iron-carbon binary phase diagram is shown in Fig. 2. Pure iron is able to form in
three allotropie variants: alpha (a), gamma (y), and delta (6). Alpha and delta iron have a
body-centered cubic (BCC) lattice structure. They are conventionally called ô ferrite or a
ferrite depending on the mode of formation. The y-Fe phase has a face-centered cubic (FCC)
lattice structure and is conventionally called austenite. The crystallographic properties of the
different allotropie forms of iron are summarized in Table 1.
Carbon atoms occupy interstitial sites in the BCC ferrite and FCC austenite unit cells,
and carbon solubility is directly related to hardening of steels. The intermetallic compound
FegC is called cementite and exists at 6.67 wt.%C with negligible solubility limits.
Cementite has an orthorhombic lattice structure and is brittle and hard. An invariant reaction
known as the eutectoid reaction results in the formation of a lamellar a+FegC structure
during cooling. This two-phase mixture is referred to as pearlite. Since the pearlitic
structure consists of soft ferrite and hard cementite layers, favorable mechanical properties
can be obtained.
MvMlU; <4 grephlU le llqeid P«
— Iree equilibria Iroa-gfsphit* equllibris
pe Weight Percent Carbon
Allotropie Forms Crystallographic
Alpha BCC 2.86 (70°F) Up to 910°C
Gamma FCC 3.65 (1800°F) 910-1403°C
Delta BCC 2.93 (2650 °F) 1403-1535°C
Density, 7.868 g/cm3 Melting point, 1535°C Boiling point, 3000°C
2.1.2. Effects of Alloying Additions on Iron-Carbon Alloys
The addition of alloying elements to the iron-carbon system affects the stability of the
phases. Additions such as Cr, Si, Al, and Mo are called ferrite stabilizers since they promote
ferrite phase formation over wider composition and temperature ranges than what are found
in the Fe-C system. At the same time, the austenite region is contracted, i.e. the y loop
shrinks. The gamma loop is seen in the Fe-Cr phase diagram in Fig. 3. In contrast, elements
such as C, Ni, Mn and N promote austenite formation and are called austenite stabilizers.
The effect of Ni on the stability of the iron phases is shown in the Fe-Ni phase diagram in Fig.
Zener and Andrews described phase stabilizing effects in terms of thermodynamic
variables. The ratio of alloying element concentrations in the a-phase (Ca) to that in the y-
phase (Cy) follows an Arrhenius-type relationship (Eq. 2).
Ça_ = ie = —+ lny9 Eq.2
where ft is a constant and A H is the enthalpy change, which is equal to the heat absorbed per
unit of solute dissolving in the y-phase minus the heat absorbed per unit of solute dissolving
in a-phase, i.e., AH=Hy-Ha. AH is positive for ferrite stabilizers since Hy is greater than Ha.
In this case, a y-loop is introduced. For the austenite stabilizers, if Hy is smaller than Ha, AH
becomes negative, and the y-region is expanded. Basic phase diagrams in terms of AH are
illustrated in Figs. 3 and 4. The relative contribution to the phase-forming strength is shown
in Fig. 5.
0 10 2000 |
o io 20 30 «0 so eo ?o aa so Weight Percent Chromium
Fig. 3. Fe-Cr phase diagram and enlarged view of gamma loop.
M 20 30 40 50 «0 70 100 0 10
Ke Weight Percent Nickel Si
Fig. 4. Fe-Ni phase diagram and enlarged view of expanded gamma region.
Fig. 5. Relative strength of alloying elements as ferrite formers and austenite formers.'41
2.1.3. Stainless Steels
Stainless steels are defined as steels that contain a Cr content greater than 10.5 wt.%
(Fig. 6). Chromium plays an important role in making the iron surface passive by forming
a Cr-rich surface oxide film that protects the underlying metal from corrosion. Stainless
steels may solidify in either austenitic or ferritic microstructures, or a combination of the two.
Intermetallic compounds (e.g., a phase) or carbides (e.g., (Fe, Cr)^C^, (Fe, Cr)7C3) may form
at intermediate temperature ranges.
Stainless steels are categorized into four groups on the basis of composition and
crystal structure: ferritic, austenitic, martensitic and duplex stainless steels. In order to
control crystal structure, the effect of ferritic and austenitic stabilizing alloying elements
should be taken into account on the basic iron-chromium system.
-140 X 10-9
2 L_ o o
Fig. 6. Corrosion rate profile with respect to Cr contents.
188.8.131.52. Ferritic Stainless Steels
Ferritic stainless steels have the BCC ferrite crystal structure as the matrix and exhibit
ferromagnetism, similar to pure iron at room temperature. These alloys contain from 12wt%
to 30wt% Cr with small amounts of minor alloying elements such as C, Mo, Si, Al, and Ti.
Since carbon is an austenite stabilizer (Fig. 5) and forms brittle carbides, the carbon content
usually remains below 0.12wt%.[2'5] In order to improve corrosion resistance, or other
properties such as weldability, other elements are added in small amounts.
The advantage of ferritic stainless steels having relatively high Cr-contents is their
excellent corrosion resistance under atmospheric, stress induced, and oxidizing environments.
However, conventional ferritic stainless steels are generally restricted in use due to poor
weldability and low ductility. Furthermore, neither heat treatment nor cold working is able to
harden ferritic stainless steels. A new generation of ferritic stainless steels, frequently
referred to as the superferritics, has been developed by reducing C and N contents. In
addition to high corrosion properties, these alloys have good ductility, formability and
184.108.40.206. Austenitic Stainless Steels
Austenitic stainless steels generally contain 16 to 25%Cr and up to around 35%Ni.
This type of alloy is so named because their structure is FCC as is y-iron. Such a structure is
obtained by adding a strong austenite stabilizer, typically Ni, to the Fe-Cr system as a
Adding austenite stabilizers, such as C, N, and Mn, can produce austenitic stainless
steels that possess outstanding mechanical properties at both cryogenic and elevated
temperatures. Figure 7 shows the yield strength of an austenitic steel (annealed Fe-18Cr-
lONi alloy) for various C+N contents as a function of temperature. Austenitic alloys can
not be hardened by heat treatment, but do harden by cold working. However, high carbon
contents can result in Cr-rich carbides forming at grain boundaries during slow cooling from
annealing temperatures. Such a grain-boundary precipitation process in a stainless steel is
generally referred to as sensitization which results in accelerated intergranular corrosion.
The critical sensitizing temperature range is from 850 down to 400°C.
A 600 -
Fig. 7. Effect of carbon and nitrogen on yield strength in the austenitic alloy.
220.127.116.11. Duplex Stainless Steels
Duplex stainless steels consist of a ferrite and austenite phase mixture. The major
alloying elements are chromium, nickel, and molybdenum, and these enable the amount of
ferrite and austenite phases to be balanced to approximately a 50-50 phase percent mixture.
Duplex stainless steels solidify 100% ferrite. Upon cooling from the melting temperature the
ferrite starts to partially decompose into austenite that nucleates and grows first at the grain
boundaries of ferrite, following favorable crystallographic orientations inside of the grains.
As the temperature lowers the ferrite content decreases as austenite increases, and carbides
and several intermetallic phases may be present. Figure 8 (a) and (b), respectively, represent
microstructures of a wrought and cast duplex stainless steel with the same composition of Fe-
22Cr-5.5Ni-3Mo-0.15N. The wrought steel exhibits a ferrite matrix with austenite islands
aligned to a certain orientation. However, the microstructure of the cast steel contains a
ferrite matrix with austenite islands of various morphologies.
The properties of duplex stainless steels are intermediate between the ferritic and
austenitic stainless steels due to the presence of dual phases. The metallurgy, properties,
alloying effects, and phase equilibria of duplex stainless steels will be discussed in detail
later in this chapter.
Fig. 8. (a) Microstructures of a wrought duplex stainless steel, parallel to rolling direction,
and (b) the cast counterpart duplex stainless steel.^
2.2.1. Factors Affecting Phase Transformations
Since most phase transformations in solids depend upon atomic movement, diffusion
is the most fundamental concept for understanding the morphologies and the kinetics of solid
phase transformations. In 1855, Adolf Pick developed equations governing diffusion that are
now known as Pick's 1st and 2nd laws of diffusion, Eq. 3 and 4, respectively. Both laws show
the relationship between diffusion and concentration gradients.
J = —D — Eq. 3 dx
ôc ô ( de L) —
ô t ô x
In these equations, D is the diffusion coefficient with typical units err?Is. The diffusion
coefficient is generally proportional to temperature and the inverse of the atomic weight.
Equation 4 is applicable to the situation where the concentration gradient changes with time
The diffusion rate is sensitive not only to the concentration gradient but also to
defects in materials such as grain boundaries, dislocations, and vacancies. Thus, the
diffusion coefficient varies with defect concentration as well as temperature. Surface and
grain boundaries are more open structures, and the resistance to atom migration is expected
to be less than inside the lattice.
Vacancies play an important role when considering substitutional diffusion. In order
to diffuse one lattice point to another, vacancies must be moving in the direction opposite to
that of atomic diffusion. For substitutional diffusion in a binary alloy system, the sum of the
A species, B species and vacancy fluxes must equal zero. In 1948, L. S. Darken^ suggested
an equation for binary interdiffusion behavior. The total flux of A atoms becomes as shown
in Eq. 5.
J A = -A, + vcA = ~ ( X b D a + X a D , ) ^ = 5^1 Eq. 5 OX ox ox
where D=XbDa+XaDb is called the interdiffusion coefficient.
18.104.22.168. Precipitate Nucleation
The first step of a phase transformation, called the nucleation process, is the
formation of small groups of atoms into stable nuclei. The driving force for nucleation is the
change in the Gibbs free energy of the system. Three different types of free energy change
can be associated with the nucleation process. Firstly, the volume free energy (AGy) of the
system is reduced with the creation of nuclei having volume V. Secondly, since nuclei create
new interfaces in contact with a supersaturated matrix, the area A of new interface increases
the free energy of the system by its surface energy, y. Thirdly, the strain field between the
matrix and nuclei due to misfit of those two phases produces a volumetric strain energy
(AGS), which increases the free energy of the system. The destruction of defects such as
grain boundaries, stacking faults and dislocations during heterogeneous nucleation process
can decrease the free energy of the system by AGd. Defects are energetically and kinetically
favored places to form nuclei. Addition of the above contributions gives the total free energy
change of the system as,
AG = -F( A G v - A G J + A y - A G d Eq. 6
For a given undercooling below the equilibrium transformation temperature, A7,
heterogeneous nucleation tends to take place at a higher rate than homogeneous nucleation.
This can in part be understood in terms of rates of diffusion, as discussed in the previous
section. Since grain boundaries are fast diffusion paths compared to the…